"the late 1890s, Hans Goldschmidt of Germany developed an aluminothermic (thermite) process for producing carbon-free chromium. Between 1904 and 1911 several researchers, particularly Leon Guillet of France, prepared alloys that would today be considered stainless steel. In 1908, Friedrich Krupp Germaniawerft built the 366-ton sailing yacht ""Germania"" featuring a chrome-nickel steel hull in Germany. In 1911, Philip Monnartz reported on the relationship between chromium content and corrosion resistance. On 17 October 1912, Krupp engineers Benno Strauss and Eduard Maurer patented austenitic stainless steel as Nirosta. Similar developments were taking place contemporaneously in the United States, where Christian Dantsizen and Frederick"
"for carbon in steel casting. Of the non-metallic elements less often recognised as metalloids, selenium—in the form of ferroselenium (50–58% selenium)—is used to improve the machinability of stainless steels. All six of the elements commonly recognised as metalloids have toxic, dietary or medicinal properties. Arsenic and antimony compounds are especially toxic; boron, silicon, and possibly arsenic, are essential trace elements. Boron, silicon, arsenic, and antimony have medical applications, and germanium and tellurium are thought to have potential. Boron is used in insecticides and herbicides. It is an essential trace element. As boric acid, it has antiseptic, antifungal, and antiviral properties."
"carbides at the grain boundaries and the strong increase in corrosion resistance made chromium an important alloying material for steel. The high-speed tool steels contain between 3 and 5% chromium. Stainless steel, the primary corrosion-resistant metal alloy, is formed when chromium is introduced to iron in sufficient concentrations, usually where the chromium concentration is above 11%. For stainless steel's formation, ferrochromium is added to the molten iron. Also, nickel-based alloys increase in strength due to the formation of discrete, stable metal carbide particles at the grain boundaries. For example, Inconel 718 contains 18.6% chromium. Because of the excellent high-temperature properties"
"phosphating), zinc and sometimes vanadium are viable substitutes. Manganese is essential to iron and steel production by virtue of its sulfur-fixing, deoxidizing, and alloying properties, as first recognized by the British metallurgist Robert Forester Mushet (1811–1891) who, in 1856, introduced the element, in the form of Spiegeleisen, into steel for the specific purpose of removing excess dissolved oxygen, sulfur, and phosphorus in order to improve its malleability. Steelmaking, including its ironmaking component, has accounted for most manganese demand, presently in the range of 85% to 90% of the total demand. Manganese is a key component of low-cost stainless steel. Often"
"special properties, such as corrosion resistance or extreme temperature stability. Manganese, silicon, or aluminium are added during the steelmaking process to remove dissolved oxygen, sulphur and phosphorus from the melt. Manganese, silicon, nickel, and copper are added to increase strength by forming solid solutions in ferrite. Chromium, vanadium, molybdenum, and tungsten increase strength by forming second-phase carbides. Nickel and copper improve corrosion resistance in small quantities. Molybdenum helps to resist embrittlement. Zirconium, cerium, and calcium increase toughness by controlling the shape of inclusions. Sulphur (in the form of manganese sulphide) lead, bismuth, selenium, and tellurium increase machinability. The alloying elements"
"its tensile strength and make the austenite form of the iron-carbon solution more stable, chromium increases hardness and melting temperature, and vanadium also increases hardness while making it less prone to metal fatigue. To inhibit corrosion, at least 11% chromium is added to steel so that a hard oxide forms on the metal surface; this is known as stainless steel. Tungsten slows the formation of cementite, keeping carbon in the iron matrix and allowing martensite to preferentially form at slower quench rates, resulting in high speed steel. On the other hand, sulfur, nitrogen, and phosphorus are considered contaminants that make"
"the greater strength of an alloy called steel. Due to its very-high strength, but still substantial toughness, and its ability to be greatly altered by heat treatment, steel is one of the most useful and common alloys in modern use. By adding chromium to steel, its resistance to corrosion can be enhanced, creating stainless steel, while adding silicon will alter its electrical characteristics, producing silicon steel. Like oil and water, a molten metal may not always mix with another element. For example, pure iron is almost completely insoluble with copper. Even when the constituents are soluble, each will usually have"
"in period 4, between chromium and iron. Manganese is often found free in nature, but is also found in combination with iron. Manganese, like chromium before it, is an important component in stainless steel, preventing the iron from rusting. Manganese is also often used in pigments, again like chromium. Manganese is also poisonous; if enough is inhaled, it can cause irreversible neurological damage. Iron (Fe) is an element in period 4, between manganese and cobalt. Iron is probably the most well-known element in period 4, being the most common element in the earth and a major component of steel. Iron-56"
"allow the moisture to collect and drop back into the food during the cooking. Although the Doufeu (literally, ""gentlefire"") can be used in an oven (without the ice, as a casserole pan), it is chiefly designed for stove top use. Stainless steel is an iron alloy containing a minimum of 11.5% chromium. Blends containing 18% chromium with either 8% nickel, called 18/8, or with 10% nickel, called 18/10, are commonly used for kitchen cookware. Stainless steel's virtues are resistance to corrosion, non-reactivity with either alkaline or acidic foods, and resistance to scratching and denting. Stainless steel's drawbacks for cooking use"
"The elastic modulus of steel is approximately 205 GPa. Steel is very prone to corrosion (rust). Stainless steel is an iron-carbon alloy with a minimum of 10.5% chromium content. There are different types of stainless steel, containing different proportions of iron, carbon, molybdenum, nickel. It has similar structural properties to steel, although its strength varies significantly. It is rarely used for primary structure, and more for architectural finishes and building cladding. It is highly resistant to corrosion and staining. Concrete is used extremely widely in building and civil engineering structures, due to its low cost, flexibility, durability, and high strength."
"and corrosion resistance. Along with the titanium alloy Ti6Al4V, 316 stainless is a common choice of material for biomedical implants. Although Ti6Al4V provides greater strength per weight and corrosion resistance, 316 stainless components can be more economical to produce. However, immune system reaction to nickel is a potential complication of 316.[1][2] Implants and equipment that are put under pressure (bone fixation screws, prostheses, body piercing jewelry) are made out of austenitic steel, often 316L and 316LVM compliant to ASTM F138.[3] 316 surgical steel is used in the manufacture and handling of food and pharmaceutical products where it is often required"
"in the production of stainless steel. In 2006 28 Mt of stainless steel were produced. Stainless steel depends on chromium for its appearance and its resistance to corrosion. The average chrome content in stainless steel is approximately 18%. It is also used when it is desired to add chromium to carbon steel. FeCr from Southern Africa, known as ""charge chrome"" and produced from a Cr containing ore with a low carbon content, is most commonly used in stainless steel production. Alternatively, high carbon FeCr produced from high grade ore found in Kazakhstan (among other places) is more commonly used in"
"niobium. Additional elements, most frequently considered undesirable, are also important in steel: phosphorus, sulfur, silicon, and traces of oxygen, nitrogen, and copper. Plain carbon-iron alloys with a higher than 2.1% carbon content are known as cast iron. With modern steelmaking techniques such as powder metal forming, it is possible to make very high-carbon (and other alloy material) steels, but such are not common. Cast iron is not malleable even when hot, but it can be formed by casting as it has a lower melting point than steel and good castability properties. Certain compositions of cast iron, while retaining the economies"
"alloying elements such as manganese, chromium, nickel, tungsten, and so on. Basically, steel is an iron-carbon alloy that does not undergo eutectic reaction. In contrast, cast iron does undergo eutectic reaction. Too little carbon content leaves (pure) iron quite soft, ductile, and weak. Carbon contents higher than those of steel make a brittle alloy commonly called pig iron. While iron alloyed with carbon is called carbon steel, alloy steel is steel to which other alloying elements have been intentionally added to modify the characteristics of steel. Common alloying elements include: manganese, nickel, chromium, molybdenum, boron, titanium, vanadium, tungsten, cobalt, and"
"A large number of other constituents may be unintentional, but benign, or may be added for other purposes such as grain refinement or corrosion resistance. In some cases, such as many aluminium alloys, an increase in strength is achieved at the expense of corrosion resistance. The addition of large amounts of nickel and chromium needed for corrosion resistance in stainless steels means that traditional hardening and tempering methods are not effective. However, precipitates of chromium, copper, or other elements can strengthen the steel by similar amounts in comparison to hardening and tempering. The strength can be tailored by adjusting the"
"both metal and non-metal, that can be added to steel to make it easier to cut. These additives may work by lubricating the tool-chip interface, decreasing the shear strength of the material, or increasing the brittleness of the chip. Historically, sulphur and lead have been the most common additives, but bismuth and tin are increasingly popular for environmental reasons. Lead can improve the machinability of steel because it acts as an internal lubricant in the cutting zone. Since lead has poor shear strength, it allows the chip to slide more freely past the cutting edge. When it is added in"
"commonly mixed with other gases, oxygen, helium, hydrogen and nitrogen. The addition of up to 5% oxygen (like the higher concentrations of carbon dioxide mentioned above) can be helpful in welding stainless steel, however, in most applications carbon dioxide is preferred. Increased oxygen makes the shielding gas oxidize the electrode, which can lead to porosity in the deposit if the electrode does not contain sufficient deoxidizers. Excessive oxygen, especially when used in application for which it is not prescribed, can lead to brittleness in the heat affected zone. Argon-helium mixtures are extremely inert, and can be used on nonferrous materials."
"Chromium Chromium is a chemical element with symbol Cr and atomic number 24. It is the first element in group 6. It is a steely-grey, lustrous, hard and brittle transition metal. Chromium boasts a high usage rate as a metal that is able to be highly polished while resisting tarnishing. Chromium is also the main component of stainless steel, a popular steel alloy due to its uncommonly high specular reflection. Simple polished chromium reflects almost 70% of the visible spectrum, with almost 90% of infrared light waves being reflected. The name of the element is derived from the Greek word"
"chromium, vanadium, molybdenum, nickel, tungsten, etc. Their alloy content raises their cost, and so they are usually only employed for specialist uses. One common alloy steel, though, is stainless steel. Recent developments in ferrous metallurgy have produced a growing range of microalloyed steels, also termed 'HSLA' or high-strength, low alloy steels, containing tiny additions to produce high strengths and often spectacular toughness at minimal cost. Apart from traditional applications, iron is also used for protection from ionizing radiation. Although it is lighter than another traditional protection material, lead, it is much stronger mechanically. The attenuation of radiation as a function"
"Maraging steel Maraging steels (a portmanteau of ""martensitic"" and ""aging"") are steels (iron alloys) that are known for possessing superior strength and toughness without losing malleability, although they cannot hold a good cutting edge. ""Aging"" refers to the extended heat-treatment process. These steels are a special class of low-carbon ultra-high-strength steels that derive their strength not from carbon, but from precipitation of intermetallic compounds. The principal alloying element is 15 to 25 wt.% nickel. Secondary alloying elements, which include cobalt, molybdenum and titanium, are added to produce intermetallic precipitates. Original development (by Bieber of Inco in the late 1950s) was"
"similar to that of Ni-based superalloys, while being far less expensive to produce. Gamma (γ): Like the phases found in Ni-based superalloys, Fe-based alloys feature a matrix phase of austenite iron (FCC). Alloying elements that are commonly found in these stainless steel alloys include: Al, B, C, Co, Cr, Mo, Ni, Nb, Si, Ti, W, and Y. While Al is introduced for its oxidation benefits, Al additions must be kept at low weight fractions (wt.%) because Al stabilizes a ferritic (BCC) primary phase matrix, which is an undesirable phase in superalloy microstructures, as it is inferior to the high temperature"
"stainless steel was introduced for the use of making appliances. This was the first material that truly replaced the usage of noble alloys in Orthodontics. Steel wire alloys, in comparison to the noble metals, were relatively cheaper. They also had better formability and can be readily used to be soldered and welded for fabrication of complex orthodontic appliances. The stainless steel alloys are of ""18-8"" austenitic type which contain Chromium (17-25%) and Nickel (8-25%) and Carbon (1-2%). Chromium in this stainless steel alloy forms a thin oxide layer which blocks the diffusion of oxygen into the alloy and allow for"
"carried out on 20 and 25 wt.% Ni steels to which small additions of Al, Ti, and Nb were made; a rise in the price of cobalt in the late 1970s led to the development of cobalt-free maraging steels. The common, non-stainless grades contain 17–19 wt.% nickel, 8–12 wt.% cobalt, 3–5 wt.% molybdenum and 0.2–1.6 wt.% titanium. Addition of chromium produces stainless grades resistant to corrosion. This also indirectly increases hardenability as they require less nickel; high-chromium, high-nickel steels are generally austenitic and unable to transform to martensite when heat treated, while lower-nickel steels can transform to martensite. Alternative variants"
"can be used un-painted. Maraging steel is alloyed with nickel and other elements, but unlike most steel contains little carbon (0.01%). This creates a very strong but still malleable steel. Eglin steel uses a combination of over a dozen different elements in varying amounts to create a relatively low-cost steel for use in bunker buster weapons. Hadfield steel (after Sir Robert Hadfield) or manganese steel contains 12–14% manganese which when abraded strain-hardens to form an incredibly hard skin which resists wearing. Examples include tank tracks, bulldozer blade edges and cutting blades on the jaws of life. Most of the more"
"low, mid and high carbon steels, with increasing carbon levels reducing ductility and toughness. The addition of silicon will produce cast irons, while the addition of chromium, nickel and molybdenum to carbon steels (more than 10%) results in stainless steels. Other significant metallic alloys are those of aluminium, titanium, copper and magnesium. Copper alloys have been known since prehistory—bronze gave the Bronze Age its name—and have many applications today, most importantly in electrical wiring. The alloys of the other three metals have been developed relatively recently; due to their chemical reactivity they require electrolytic extraction processes. The alloys of aluminium,"
"Austenitic stainless steel Austenitic stainless steel is a specific type of stainless steel alloy. Stainless steels may be classified by their crystalline structure into four main types: ""austenitic"", ""ferritic,"" ""martensitic and duplex."" These stainless steels possess austenite as their primary crystalline structure (face centered cubic). This austenite crystalline structure is achieved by sufficient additions of the austenite stabilizing elements nickel, manganese and nitrogen. Due to their crystalline structure austenitic steels are not hardenable by heat treatment and are essentially non-magnetic. There are two subgroups of austenitic stainless steel. 300 series stainless steels achieve their austenitic structure primarily by a nickel"
"out of the melt and into the slag. The amount of manganese required to neutralize sulfur is 1.7 × sulfur content + 0.3%. If more than this amount of manganese is added, then manganese carbide forms, which increases hardness and chilling, except in grey iron, where up to 1% of manganese increases strength and density. Nickel is one of the most common alloying elements because it refines the pearlite and graphite structure, improves toughness, and evens out hardness differences between section thicknesses. Chromium is added in small amounts to reduce free graphite, produce chill, and because it is a powerful"
"in order to minimize metallic contamination. ASTM F138[3]-compliant steel is also used in the manufacture of body piercing jewellery[4] and body modification implants. 440 and 420 stainless steels, known also by the name ""Cutlery Stainless Steel"", are high carbon steels alloyed with chromium. They have very good corrosion resistance compared to other cutlery steels, but their corrosion resistance is inferior to 316 stainless. Biomedical cutting instruments are often made from 440 or 420 stainless due to its high hardness coupled with acceptable corrosion resistance. Long story short, not all ""surgical stainless steel"" is safe for initial or healed piercings. Your"
"to produce the combination of low carbon and high chromium found in most modern stainless steels, and the high-chromium alloys they could produce were too brittle to be practical. It was not until 1912 that the industrialisation of stainless steel alloys occurred in England, Germany, and the United States. By 1900 three metals with atomic numbers less than lead (#82), the heaviest stable metal, remained to be discovered: elements 71, 72, 75. Von Welsbach, in 1906, proved that the old ytterbium also contained a new element (#71), which he named ""cassiopeium"". Urbain proved this simultaneously, but his samples were very"
"Carbon additive Carbon additive is a product that is added to molten steel. Carbon additive includes calcined petroleum coke, graphite petroleum coke, calcined anthracite coal, electrical calcined anthracite, and natural graphite. For the steel-making industry, the most suitable carbon additive is calcined petroleum coke with fixed carbon of 98.5%min. Sulfur in calcined petroleum coke is a crucial element, for sulfur impacts the quality of steel. The lower the sulfur, the better quality of calcined petroleum coke. The sulfur content of calcined petroleum coke is decided by the sulfur content in petroleum coke. Northeast China is the only source of low"
"Stainless steel fiber Stainless steel fibers are manufactured fibers composed of stainless steel. Composition may include carbon (C), silicon (Si), manganese (Mn), phosphorus (P), sulfur (S), and other elements. Currently stainless steel fibers are manufactured primarily in Europe. The most common uses for stainless steel fibers is in the field of the electrical and textiles industry such as anti-radiation cloth, thermal resistant fabric, and anti-static brushes. Many people also use stainless steel fibers in weaving. Increasingly common today are stainless steel fibers in clothing, including radiation protection for pregnant women. Stainless steel yarns are woven, braided, and knit into many"
"their high chromium content, certain D-type tool steels are often considered stainless or semi-stainless, however their corrosion resistance is very limited due to the precipitation of the majority of their chromium and carbon constituents as carbides. ISO 1.2767, also known as DIN X 45 NiCrMo 4, AISI 6F7, and BS EN 20 B, is an air-hardening tool steel with a primary alloying element of nickel. It possesses good toughness, stable grains, and is highly polishable. It is primarily used for dies in plastic injection molding application that involve high stresses. Other applications include blanking dies, forging dies, and industrial blades."
"allows the elimination of most natural and foreign inclusions from the metal. However its general content in different steels can vary between wide limits and has a big influence on the metal properties. Non-metallic inclusions, the presence of which defines purity of steel, are classified by chemical and mineralogical content, by stability and by origin. By chemical content non-metallic inclusions are divided into the following groups: The majority of inclusions in metals are oxides and sulfides since the content of phosphorus is very small. Silicates are very detrimental to steels, especially if it has to undergo heat treatment at a"